CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 Contents lists available at ScienceDirect CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry journal homepage: www.elsevier.com/locate/calphad Thermodynamic assessment of the cesium–oxygen system by coupling density functional theory and CALPHAD approaches C. Guéneau n, J.-L. Flèche CEA Saclay, DEN, DPC, SCCME, F-91191 Gif-sur-Yvette, France art ic l e i nf o a b s t r a c t Article history: Received 17 September 2014 Received in revised form 13 February 2015 Accepted 18 February 2015 Available online 3 March 2015 The thermodynamic properties of cesium oxides were calculated by combining ab initio calculations at 0 K and a quasi-harmonic statistical thermodynamic model to determine the temperature dependency of the thermodynamic properties. In a second approach, the CALPHAD method was used to derive a model describing the Gibbs energy for all the cesium oxide compounds and the liquid phase of the cesium– oxygen system. For this approach, available experimental data in the literature was reviewed and it was concluded that only experimental thermodynamic data for Cs2O are reliable. All these data together with the thermodynamic data calculated by combining ab initio and the statistical model were used to assess the Gibbs energy of all the phases of the cesium–oxygen system. A consistent thermodynamic model was obtained. The variation of the relative stability of the different oxides is discussed using structural and bond data for the oxides investigated by ab initio calculations. This work suggests that the melting point for Cs2O2 reported in the literature (863 K) is probably overestimated and should be re-measured. & 2015 Elsevier Ltd. All rights reserved. Keywords: Cesium oxides Thermodynamics Computational modeling CALPHAD – ﬁrst-principle calculations Quasi-harmonic model 1. Introduction The ﬁssion of uranium–plutonium mixed oxide fuel in nuclear reactors produces many ﬁssion products and results in an increase in the oxygen potential of the fuel, which is a key thermodynamic data for nuclear fuels. Cesium is one of these major ﬁssion products. It can form ternary oxide phases such as CsxUyOz, CsxMoyOz, etc. in the fuel. When cesium combines with other elements, such as I, Te, O, it can be responsible for the chemical attack of steel claddings . The fuelbase thermodynamic database is being developed in CEA since 2005 as a computational tool to perform thermodynamic calculations on mixed oxide fuels containing ﬁssion products to simulate the chemistry of the irradiated fuel [2– 5]. In 2013, the TAF-ID project was launched to develop the same kind of database in frame of an international collaboration within the OECD/NEA [www.oecd-nea.org/science/taf-id/]. The system Cs–O is a key system required to model and investigate important ternary systems (e.g., U–Cs–O, Cs–Te–O, Cs–Mo–O, etc.). This paper presents a review of available data in the literature and a thermodynamic assessment developed with the CALPHAD method on the basis of both selected experimental data coming from the literature as well as thermodynamic data for the cesium oxides calculated by combining ab initio calculations and a quasi-harmonic statistical model (present work). Experimental data n Corresponding author. E-mail address: [email protected] (C. Guéneau). http://dx.doi.org/10.1016/j.calphad.2015.02.002 0364-5916/& 2015 Elsevier Ltd. All rights reserved. available in the literature are ﬁrst reviewed. Then the method to calculate the thermodynamic functions for the different cesium oxides using ab initio calculations and the quasi-harmonic model is brieﬂy described (complete method is discussed in Ref. ). Finally the thermodynamic assessment using all these data is presented. 2. Review of literature data Numerous oxide compounds are reported to exist in the Cs–O system: Cs7O, Cs4O, Cs7O2 (or Cs11O3), Cs3O, Cs2O, Cs2O2, CsO2, Cs2O3, and CsO3. Thermodynamic and phase equilibria data available in the literature on the Cs–O system are summarized in Table 1. Thermodynamic data for cesium oxides were compiled and critically evaluated by Lamoreaux and Hildenbrand  and later by Cordfunke and Konings . In this section, the available experimental data are reviewed. 2.1 Phase diagram data Only limited studies were undertaken on the Cs–O system by Rengade , Brauer  and Knights and Phillips . The most recent version of the phase diagram published by Cordfunke and Konings  and later by Okamoto  was based on the experimental study performed by Knights and Phillips . Among the different compounds, the existence of Cs2O3 is not well established. 68 C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 Table 1 Available experimental thermodynamic and phase diagram data on the Cs–O system Type of data Composition, temperature range (K) Method Reference Phase diagram Phase diagram Phase diagram Phase diagram Phase diagram Phase diagram Oxygen pressure Oxygen potential Heat capacity Oxygen pressure Cs pressure Enthalpy of formation Enthalpy of formation Cs–Cs2O, 250–500 K Cs–Cs2O, 250–500 K Cs–CsO2, 250–500 K Melting point CsO2 Melting point CsO2 Melting point Cs2O Cs2O2 þ CsO2, Cs2O2 þ Cs2O, 593–713 K 3.3–17 at% O, 773–973 K Cs2O, 5–350 K Cs2O2, 573–613 K Cs-Cs2O, 553–653 K Cs2O, 298.15 K Cs2O, 298.15 K Thermal analysis Thermal analysis Differential scanning calorimetry Rengade  Brauer  Knights and Philips  Blumenthal  Vol’nov  Differential thermal analysis, thermogravimetry, X-ray diffraction Touzain  Manometerþbalance Berardinelli [15,16] Electromotive Force Measurement Knights and Philips  Adiabatic calorimetry Flotow and Osborne  Morris  Membrane sensor Arnol’dov  Solution calorimetry Settle  Solution calorimetry Beketov  In the Cs–Cs2O part, an eutectic reaction (liquid¼ Cs bccþ Cs7O) was measured by Brauer  at 271 K and the compound Cs7O was found to melt congruently at 276 K. The measurements performed by Knights and Phillips  using a differential scanning calorimeter lead to some modiﬁcations of Brauer's version in the region from Cs7O to Cs7O2. An eutectic reaction (liquid¼Cs7OþCs4O) was measured by Knights and Phillips  at 262 K. Their observation of a transition at 262.7 K between 20 and 25 at% O implies that Cs7O2 decomposes by a peritectic reaction into Cs7O and Cs3O. Cs4O was found to decompose at 326 K into liquid and Cs3O. And Cs3O was observed to decompose into liquid and Cs2O at 437 K. The melting point of Cs2O was found at 768 K by Touzain  using DTA. The investigation of the Cs2O–CsO2 region by Knights and Phillips  highlighted difﬁculties to obtain reproducible results on phase transitions due to a chemical interaction between the containment materials and samples. The melting points for Cs2O2 and CsO2 and the decomposition temperature of CsO3 are quite uncertain and only indicative. The melting point of CsO2 was estimated at 705 K by Blumenthal and Centerszwer  and later reported as 723 K by Vol’nov . The largest uncertainties were on both the melting point of Cs2O2 (863 K) and the decomposition of CsO3 (343 K), which were reported on the phase diagrams successively by Knights and Phillips , Cordfunke and Konings . In fact, the original paper with the measurements and the details on the method, cited by the above authors, could not be found in the literature. To conclude, the phase equilibria are relatively well established in the Cs–Cs2O portion of the diagram. On the contrary, the Cs2O– O region is not well known and remains uncertain due to difﬁculties encountered during experimentation (e.g., chemical interaction between samples and crucibles). 2.2 Thermodynamic data 2.2.1. Oxygen and cesium potential data The thermal decomposition of CsO2 and Cs2O2 oxides was investigated by Berardinelli  in the temperature range (633– 723 K) using a manometer and a balance to determine the total pressure (O2) and oxygen to metal ratio. The overall composition of the samples fabricated from CsO2 decomposition lied in the two-phase region (Cs2O2 þCsO2) according to the reaction (2CsO2(s) ¼Cs2O2(s) þO2(g)). CsO2 was observed to start to melt at 723 K in agreement with Vol’nov . Measurements were carried out both below and above the melting temperature. Data measured in (Cs2O2 þCsO2) by Berardinelli  compare very well with Morris’s data . From the measurements above the melt (733–773 K), two regions were proposed: a single liquid phase and a two-phase (liquid þCs2O2) region. The liquidus composition in Remark Not used Selected Selected Not used Selected Selected Selected Selected Selected Not used Not used Selected Not used this temperature range was estimated to be Cs2O3.32. Nevertheless the liquidus composition was found to be constant with temperature, which is not expected. The decomposition of Cs2O2 according to the reaction (2Cs2O2(s) ¼2Cs2O(s) þO2(g)) was investigated over the temperature range (600–773 K) leading to sample composition ranging between Cs2O1.15 and Cs2O1.94 in the two-phase region (Cs2O þCs2O2). Pressure data measured by Morris  are slightly lower than those of Berardinelli . The measurements performed by Berardinelli in  on the thermal decomposition of Cs2O2 and CsO2 were later published in  in which experimental data measured above the melt were not reported. Arnol’dov et al.  performed static measurements of total pressure (Cs) above Cs–Cs2O mixtures (with compositions ranging from 0 to 18.7 at% O). Pure cesium was taken as the standard state to determine activities. Pure cesium pressure data were found to be 15–20% higher than previous measurements. A comparison of data for pure cesium from Arnol’dov et al.  and from Hill and Gotoh  shows a large discrepancy between the two datasets. Oxygen potentials in Cs–O liquids with 3.3–17 at% O at 773– 973 K were determined by Knights and Phillips  from EMF measurements using ThO2–10 mol% Y2O3 electrolyte. Cesium potentials were derived at 773 K using the Duhem–Margules equation. Knights and Phillips  have extrapolated oxygen and cesium potentials from 17 to 66 at% O as well as the Gibbs energy of formation of Cs2O, Cs2O2, and CsO2 by combining their own measurements and data measured by Berardinelli and Kraus . Knight and Phillips  compared their calculated Cs potentials using Gibbs-Duhem with experimental data derived by Arnol’dov et al. . A good agreement was found except for the highest oxygen content (17.5 at% O). This disagreement could be due to a reaction with the reactor vessel according to Knight and Phillips . As vapor pressure data for pure cesium from Arnol’dov et al.  are in disagreement with other data in the literature, the Cs potentials derived by Knight and Phillips  are preferred in the present work. 2.2.2. Enthalpy, entropy and heat capacity data Cs2O is the only compound for which a reliable enthalpy of formation is available. In fact, the enthalpy of formation of Cs2O(s) was measured by Beketov , Rengade , and Settle et al.  at room temperature using solution-calorimetry from the enthalpy of reaction of Cs2O(s) with excess water from CsOH(aq). As recommended by Cordfunke and Konings , data measured by Settle et al.  is preferred: ΔH0f (Cs2O at 298.15 K)¼ 345.9871.17 kJ/mol. The heat capacity of Cs2O(s) was measured using adiabatic calorimetry from 5 to 350 K by Flotow and Osborne . Thermodynamic data at room temperature and H0 (298.15 K)–H0 C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 (0) were obtained from these measurements: Cp0(Cs2O) (J mol 1 K 1)¼ 66.024þ0.033461n(T/K), F = − Ecohesive (V ) ⎡ 9 + Nk B T ⎢ x D + 3ln (1 − e−x D ) − D (x D ) ⎢⎣ 8 S0 (Cs2O at 298.15 K) ¼ 146.87 70.44 (J mol 1 K 1) 3n − 3 ∑ + The authors have extrapolated the heat capacity data up to 763 K and derived the Gibbs energy of formation using the enthalpy data of Settle et al. . The Gibbs energy of formation of Cs2O, Cs2O2, and CsO2 was derived by Knights and Phillips  from oxygen and cesium potential data reported by Berardinelli and Kraus : ΔGf (Cs2O2) (J mol 1) ¼ 390,052 þ201.7n(T/K). By the same method, Knights and Phillips  derived the Gibbs energy of formation of CsO2: ΔGf (CsO2) (J mol 1)¼ 233,145þ 153.65n(T/K). Lindemer et al.  did their own assessment. Their data for Cs2O2 and CsO2 are in disagreement with the oxygen potential data from Berardinelli and Kraus . Thermodynamic data for Cs2O, Cs2O2 and CsO2 compounds have been determined by Lamoreaux and Hildenbrand  on the basis of available experimental data as well as analogy with Na–O system. The authors have estimated the melting enthalpy of Cs2O, Cs2O2, and CsO2 too. The selected experimental data for the thermodynamic assessment using the CALPHAD method are reported in Table 1. j=1 i. The adiabatic approximation to calculate the cohesive energy of the crystal Ecohesive versus static pressure at zero kelvin, and correspondingly versus the equilibrium volume. ii. The harmonic approximation to calculate the 3n vibration fre→ → quencies νj( q ) (j¼1,3n) for N values of wave vector q in the ﬁrst Brillouin zone. These 3n frequencies dispersion branches are divided into three acoustic branches and (3n 3) optical branches. In order to make ab initio computations tractable, these vibration frequencies are calculated at the Γ point only → → ( q = 0). For q ≠ 0 we use the Debye model to determine the acoustic vibration frequencies and the Einstein model for the optical vibration frequencies. From Ecohesive (V) and the fre→ quencies νj( q ¼ 0) (j¼1,3n) it is possible to construct the partition function of the crystal and deduce its free energy at temperature T by the statistical thermodynamic laws: (1) −1/3 1/2 ⎛ 1/2 ⎛ 2 − 2σ 0 ⎞3/2⎞ h ⎛ 9 ⎞1/3 ⎛ B ⎞ ⎛ 1 − σ 0 ⎞ ⎜ ⎟ ⎟ ⎟ ⎜ ⎟ ⎜3 ⎟ ⎜ ΘD = 1 + 2⎜ k B ⎝ 4π V ⎠ ⎝ ρ ⎠ ⎝ 1 + σ 0 ⎠ ⎜ ⎝ 1 − 2σ 0 ⎠ ⎟⎠ ⎝ (2) B is the bulk modulus, ρ is the density, and s is the Poisson ratio (close to 0.33). iii. To account for the thermal expansion while maintaining the simplicity of the harmonic model, quasi-harmonic approximation is used assuming that the vibration frequencies change with the volume of the unit cell: 0 pV = V ⎡ ⎛9 ⎞ dEcohesive (V ) + Nk B T ⎢γacoustic ⎜ x D + 3D (x D ) ⎟ ⎝8 ⎠ ⎢⎣ dV 3n − 3 + γoptic ∑ j=1 xj ⎛xj ⎜ + x j ⎝2 e − ⎞ ⎤⎥ ⎟ 1 ⎠ ⎥⎦ (3) where γacoustic and γoptic are the Gruneïsen coefﬁcients. For an ideal isotropic crystal these Gruneïsen coefﬁcients are given by  3. Ab-initio calculations combined with a quasi-harmonic model The thermodynamic functions of the CsxO2y compounds can be calculated starting from the free energy modeled at quasi-harmonic approximation level and with the assistance of ab initio calculations . The advantage of this approach is that it does not require any parameter to perform the calculations except the symmetry group, the lattice parameters of the unit cell, and the atom position coordinates. To determine the free energy of a crystal, containing N cells of n atoms per cell, the following three approximations are mainly used: ⎛xj ⎞⎤ ⎜ + ln (1 − e−x j ) ⎟ ⎥ ⎝2 ⎠ ⎥⎦ where xj ¼ hνj(0)/kBT. D(xD) is the Debye function with xD ¼ ΘD/T where ΘD is the Debye temperature. kB and h are the Boltzmann and Planck constants, respectively. For an ideal isotropic crystal  ΘD is given by γacoustic = − 3.1. Method to calculate the thermodynamic functions 69 γoptic = 2 1 d ⎛ d2Ecohesive (V ) ⎞ ⎟⎟ − V ln ⎜⎜ 3 2 dV ⎝ dV 2 ⎠ 1 d ⎛ d2Ecohesive (V ) ⎞ ⎟⎟ V ln ⎜⎜ 2 dV ⎝ ⎠ dV 2/3 (4) (5) The volume V is calculated iteratively for a given pressure and temperature, knowing Ecohesive(V) and the vibration frequencies at Γ point, as well as the Poisson ratio s0 for the crystal to zero static pressure. From F(T, V) and pV we can calculate the entropy S¼ (dF/dT)V, the internal energy U¼FþTS, the heat capacity at constant volume Cv ¼(dU/dT)V, the bulk modulus B¼ V(dp/dV)T, the thermal expansion αp ¼(dp/dT)V/B, and the heat capacity at constant pressure Cp ¼ Cv þTVBα2. The calculation of the thermodynamic functions in the standard conditions is carried out with this approach, for the suboxides Cs7O, Cs4O, Cs11O3, Cs3O, the normal oxide Cs2O, the peroxide CsO (or Cs2O2), the superoxide CsO2, and the cesium ozonide CsO3. 3.2. Results The most studied cesium oxides, in the literature, from the point of view of their electronic structure calculation are Cs2O [25– 28], Cs2O2 [25,27,28] and CsO2 [25,27–29]. Ab initio calculations were also performed for Cs11O3, Cs3O, CsO3 in . These results were obtained with different codes using the electronic density functional theory (DFT) with a plane-wave pseudo-potential method. The results of the formation enthalpy at 0 K obtained by these authors are reported in Table 5. In the present work, our calculations were performed with the CASTEP code , which solves the electronic Schrödinger equation for a compound with periodic lattice, within the electronic 70 C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 density functional theory (DFT) with a plane-wave pseudo-potential method. The tightly bound core electrons are represented by non local ultrasoft pseudo-potentials as proposed by Vanderbilt . The exchange/correlation energies are calculated using the Perdew–Wang form of the generalized gradient approximation . Due to the presence of oxygen, the cutoff energy is taken to 430 eV throughout all the calculations. The ﬁrst Brillouin zone is approximated with ﬁnite sampling of k-points using the Monkhorst–Pack scheme . Futhermore, when the electron spins of the ions are unpaired, the calculations are carried out with polarized spins. For CsO (Cs2O2), which contains the peroxide ion O22−, all the spins are paired. This is not the case for CsO2 and CsO3, which contain an unpaired spin due to the presence of superoxide ion O2− and ozonide ion O3−, respectively. The spin polarization calculation with the symmetric group (I4/mmm) for CsO2 and (P21/c) for CsO3 opens an energy gap for CsO3, but not for CsO2. Experimental investigations and DFT calculations by Riyadi et al.  show that the symmetry group of CsO2 is lower than I4/mmm. To take into account the antiferromagnetic order proposed by the authors and open an energy gap, CsO2 material is studied with the I41/a symmetry group with unit cell dimensions corresponding to 2a, b and 2c of the original cell. The set of parameters required for completing these ab initio calculations and the results obtained for the structure at zero pressure are listed in Table 2. As shown in Table 2, the c parameter of the normal oxide Cs2O is much larger than the lattice parameter of the reference structure, inducing a relative error of 23% on the equilibrium volume. In fact, the hexagonal unit cell of Cs2O contains three triple layers Cs– O–Cs weakly bonded together through Van der Waals interactions . Unfortunately, the correct long-range effect of such interaction is absent from gradient corrected exchange-correlation functional in density-functional theory. To overcome this shortfall and obtain an improved result for the c parameter and volume (see Table 2), a special hybrid semi-empirical solution was applied. Such a modiﬁcation allows the CASTEP code to introduce damped atom-pairwise dispersion corrections of the form C6R 6 in the DFT formalism . These corrections were also applied for CsO3 as a small increase in volume was initially calculated. Using the total energy for cesium oxides for a given pressure and the energy of pure cesium and oxygen atoms as references, also calculated with the CASTEP code, we obtain the cohesive energy Ecohesive of the crystal as a function of the static pressure or the corresponding equilibrium volume V. To calculate the standard enthalpy of formation ΔHf (T) we use Hess's law. Beside the reaction of formation of the cesium oxide from the pure components in their standard states, we consider the reaction of sublimation for cesium and dissociation of oxygen in atomic gas phase followed by the reaction of formation of the oxide from these gases, which is the reversed reaction of “atomisation”: xCscrystal + yO2gas → Cs x O2ycrystal ( ΔHf Cs x O2ycrystal xCscrystal + yO2gas → xCsgas + 2yOgas xCsgas + 2yOgas → Cs x O2ycrystal ) xΔHf (Csgas) + 2yΔHf (Ogas ) ( –ΔHatomisation Cs x O2ycrystal ) We obtain at temperature T: ΔHf (CsxO2crystal ) = xΔHf (Cs gas) y + 2yΔHf (O gas) −ΔHatomisation(CsxO2crystal ) y (6) Table 2 Parameters and results of the ab initio calculations with the CASTEP Code. DFT lattice parameters (Å) and equilibrium volume of unit cell (Å3), in italic, at zero pressure, are compared to experimental data from Ref. . Volume(Å3) Exp.  DFT calc. Relative error Metal or insulator 9.193 9.357 2139.46 2183.46 (2%) 4293.35 4496.23 (5%) 3842.55 4035.98 (5%) 502.04 523.17 (4%) 297.03 365.20 (23%) 290.57 ( 2%) 208.90 221.43 (6%) 1166.85 1215.72 (4%) 323.56 360.51 (11%) 338.70 (5%) Metal Symmetry group Exp.  Magnetism Monkhorst–Pack scheme a (Å) Exp.  DFT calc. Cs7O Hex. P-6m2 no 8 8 12 16.393 16.414 Cs40 Orth. Pna21 no 659 16.833 17.027 20.569 20.882 12.400 12.643 Cs11O3 Mono. P21/c no 483 17.610 17.880 9.218 9.377 β(100.14/100.29) 24.047 24.466 Cs3O Hex. P63/mcm no 999 8.780 8.899 7.520 7.627 Cs2O Trig. R-3m no 11 11 3 4.269 4.330 18.820 22.491 4.232 18.74 with dispersion correction CsO Orth. Immm no 10 6 7 4.322 4.460 CsO2 Tetrag. I41/a (2a, b, 2c) AFM 664 8.924 9.031 CsO3 Mono. P21/c FM 775 6.709 7.008 With dispersion correction 6.836 b (Å) Exp.  DFT calc. β (exp/calc.) c (Å) Exp.  DFT calc. Oxide 7.517 7.644 6.430 6.495 14.652 14.906 6.244 6.556 β(120.85/123.61) 6.358 β(120.85/122.41) 8.997 9.420 9.231 Metal Metal Metal Insulator Insulator Insulator Insulator C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 ΔHf(Csgas) and ΔHf(Ogas) are known and ΔHatomisation(CsxO2ycrystal) is given by the model tabulated. dEcoh (V ) 5 + nNk B T dV 2 ⎡ ⎛9 ⎞ − Nk B T ⎢ (γac + 1) ⎜ x D + 3D (x D ) ⎟ + (γop + 1) ⎝8 ⎠ ⎢⎣ 3n − 3 ∑ j=1 4. CALPHAD assessment of the Cs–O system The models to describe the Gibbs energies for all the phases are ﬁrstly described. Then the optimization procedure is explained and ﬁnally, the results are presented and compared to available experimental data and to calculated data for the compounds using DFT and the quasi-harmonic model. ) ΔHatomisation (Cs x O2crystal y = Ecohesive (V ) + V 71 4.1. Models x j ⎞⎤ ⎛xj ⎟⎥ ⎜ + x j ⎝2 e − 1 ⎠ ⎥⎦ (7) The calculated enthalpy of formation ΔH0f, entropy S0 and heat capacity at constant pressure Cp0 at 298.15 K and 1 atm for all the CxO2ycrystal compounds are compared with experimental and assessed data using CALPHAD in the next section (Table 5). Concerning the heat capacity data at constant pressure, the following regression law is used: Cp (J·mol−1·K −1) = k 0 + k2 T 2 + k1T + k−2 T −2 (8) This mathematical function used in the CALPHAD models (Eq. (19)) is generally valid from 298.15 K to the melting point of the pure elements or compounds. In case of cesium with a low melting point at 300 K, the SGTE function from Dinsdale  used in our CALPHAD model is valid for T4 200 K. Thus, we will consider that for all the compounds, our CALPHAD models are valid from temperatures higher than 200 K, which is consistent with the experimental phase diagram data  given for T4200 K. Heat capacity data calculated with the quasi-harmonic model are compared with experimental data measured by Flotow and Osborne  from 5 to 350 K for the Cs2O compound in Fig. 3(e). In fact, this is the only compound for which experimental heat capacity data are available. The agreement is good with a deviation of 1.6% at 300 K. Thus, we consider that our approach (DFTþ quasiharmonic model) is validated. Nevertheless, for this compound, we chose to ﬁt existing experimental data instead of the theoretical data because we consider that these experimental data are more accurate. Data at higher temperature from the literature are extrapolated. For the other compounds Cs7O, Cs4O, Cs11O3, Cs3O, Cs2O2, CsO2, and CsO3 no experimental data exists. Therefore, the ki coefﬁcients were assessed by ﬁtting quasi-harmonic model data. The results are shown in Fig. 3(a)–(d) and (f)–(h). The ki coefﬁcients are listed in Table 3 for all the compounds. A very good agreement is obtained for temperatures above 200 K. A comparison between all data will be presented in the next section. All the Gibbs energies are referred to the Standard Element Reference (SER) state corresponding to HiSER , the enthalpy of the pure element in its stable state at 298.15 K and 1 atm. 4.1.1. Pure elements The Gibbs energy function 0Giφ (T ) = Giφ (T ) − HiSER for the element i in the phase φ is expressed as 0 φ Gi (T ) = a + b⋅T + c⋅T ⋅ ln T + dn ⋅T n (9) with n ¼2, 3, 1. The Gibbs energies for pure Cs and O were taken from Dinsdale . 4.1.2. Liquid phase A two-sublattice ionic liquid model (Cs þ )P(O 2,Va Q,CsO2,O)Q was used to describe the liquid phase . The model assumes that cations are in the ﬁrst sublattice and that anions and neutral species mix in the second sublattice. Hypothetical charged vacancies (Va Q) allow the neutrality of the system from the pure metal to the liquid oxides to be maintained. P and Q are the average charges of the ﬁrst and second sublattices, respectively. For the Cs–O system, P and Q are equal to P = 2y O2 − + y Va−1 (10) Q=1 (11) where yO2− and y Va1− designate site fraction of oxygen and vacancies respectively in the second sublattice. A ﬁrst attempt was made to describe the liquid phase with the simplest sublattice model (Cs þ )P(O 2,Va Q,O)Q without associate species (CsO2). With this model, it was not possible to get a correct shape of the liquidus from Cs2O to O. Thus, the (CsO2) associate was added in the second sublattice. This species was preferred to (Cs2O2) due to the too large uncertainty on its melting point. The Gibbs energy of the liquid phase is expressed as G liq = ref G liq + idG liq + ex G liq (12) Table 3 Regression coefﬁcients to ﬁt the theoretical heat capacity data in J mol 1 K 1 of cesium oxides versus temperature at constant pressure valid from 298.15 K to the melting point. For Cs2O, experimental data were used. Oxide k0 k1 k2 k-2 Cs7O Cs40 Cs11O3 Cs3O Cs2O Cs2O2 CsO2 CsO3 0.18896318E þ 03 0.11984977E þ 03 0.33608049E þ03 0.63382374E þ 02 0.690158626E þ 02 0.84555089E þ 02 0.62655412E þ 02 0.63382374E þ 02 0.74629283E 01 0.33404469E 01 0.89345443E 01 0.72948843E 01 0.2700182E 01 0.3563614E 01 0.22489574E 01 0.72948843E 01 0.11007908E 05 0.95651960E 06 0.23205005E 05 0.11304622E 05 0.37243959E 05 0.38732760E 05 0.48403552E 06 0.11304622E 05 0.78549294E þ05 0.10465812E þ 06 0.31196982E þ 06 0.72192385E þ 05 0.8926800E þ 05 0.121432E þ 06 0.76811847E þ 05 0.72192385E þ 05 72 C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 Table 4 Assessed thermodynamic parameters for the phases of the Cs–O system (J mol 1). Phase Gibbs energy parameters (J mol 1) Reference Liquid (Cs þ )P(O2 ,Va Q,CsO2,O)Q 0 This work G liq + (Cs )2 (O2 −) 0 = 0G Cs2O + 25,799.2 − 33.592632 T  G liq + (Cs )(Va−) 0 2) 0  G(liq O) L 0 + 2− (Cs )(O , Va) = − 29,927 + 5.4535 T This work L1 = − 4978 + 9.926 T This work L2 = 6971 This work (Cs+)(O2 −, Va) (Cs+)(O2 −, Va) = 7000 This work = − 30,000 This work L 0 + 2− (Cs )(O , CsO2) L0 (Cs+)(CsO2, O) Cs7O This work = 0G CsO2 + 24,942 − 32 T liq G (CsO 0 Cs7O G This work = − 400,474 + 663.75459 T − 188.96318 T ln (T ) − 0.037314641 T 2 − 1.8346513 × 10−7 T 3 + 39275 T (−1) Cs4O 0 Cs4 O G This work = − 376,829 + 449.05376 T − 119.84977 T ln (T ) − 0.016702234 T 2 − 1.5941993 × 10−7 T 3 + 52329 T (−1) Cs7O2 0 Cs7O2 G − 2.48625 × Cs3O 0 Cs3O G This work = − 750,000 + 843.9 T − 216.051744 T ln (T ) − 0.028718178 T 2 10−7 T3 + 100,276 T (−1) This work = − 371,929 + 388.84685 T − 95.926195 T ln (T ) − 0.012825603 T 2 − 1.3849564 × 10−7 T 3 + 42,364 T (−1) Cs2O 0 Cs2O G + 6.2073265 × Cs2O2 This work = − 368,025 + 323.73258 T − 69.0158626 T ln (T ) − 0.0135009113 T 2 0 Cs2O2 G 10−7 T3 + 44,634 T (−1) This work = − 417,219 + 362 T − 84.555089 T ln (T ) − 0.01781807 T 2 + 6.45545997 × 10−7 T 3 + 60,716 T (−1) CsO2 0 CsO2 G This work = − 261,350 + 263.5 T − 62.655412 T ln (T ) − 0.011244787 T 2 + 8.0672586 × 10−8 T 3 + 38,406 T (−1) CsO3 0 CsO3 G + 1.8841036 × 10−7 T3 + 36,096 with ref G liq = y O2 − 0 G liq + (Cs ) 2 (O 2 −) 0 liq liq + yVa 0 G (Cs +)(Va−) + yCsO2 G (CsO2) + yO 0 G (liq O) (13) ( id G liq = QRT y O−2 ln y O−2 + yVa ln yVa + yCsO2 ln yCsO2 + yO ln yO ex G liq = y O2 − yVa L liq + (Cs )(O 2 −, Va) ) (14) + y O2 − yCsO2 L liq + (Cs )(O 2 −, CsO2) liq + y O2 − yCsO2 L (Cs +)(CsO2, O) (15) with L liq + 2 − (Cs )(O , Va) = L 0 + 2− (Cs )(O , Va) + (y O2 − − ) yVa L 1 + 2 − (Cs )(O , Va) 2 + (y O2 − − yVa ) L 2 (Cs+)(O 2 −, Va) L liq + (Cs )(O 2 −, CsO2) = L0 (Cs+)(O 2 −, CsO2) liq 0 L (Cs +)(CsO2, O) = L (Cs+)(CsO2, O) This work = − 295,000 + 278 T − 63.382374 T ln (T ) − 0.036474421 T 2 (16) (17) T (−1) 4.1.3. Solid oxide compounds Cs7O, Cs4O, Cs7O2, Cs3O, Cs2O, Cs2O2, CsO2 and CsO3 oxides are described as stoichiometric compounds. The Gibbs energy function for a CsnOm compound referred to the standard enthalpy of the elements is expressed by 0 SER GiCsn Om (T ) − n⋅HCs − m⋅HOSER = a + b⋅T + c⋅T ⋅ ln T + dn ⋅T n (19) with n¼ 2, 3, 1. For Cs7O2 compound data, which was reported on the phase diagram and chosen in the CALPHAD assessment, the DFT calculations were performed on Cs11O3 and then rescaled by multiplying by a factor of (9/14). 4.1.4. Gas phase The gas is described as an ideal mixture of the following species: (Cs, Cs2, Cs2O, Cs2O2, O, O2, O3) The Gibbs energy is expressed by ⎤ ⎡ G gas = ∑ yi ⎢⎢0 Gigas i ⎣ − ⎛p⎞ ⎟⎟ ⎝ p0 ⎠ + RT ln yi ⎥ + RT ln ⎜⎜ ∑ bij H SER j ⎥ j ⎦ (20) (18) where the interaction coefﬁcients Li with i¼0, 1, 2 can have a linear dependence with temperature. Interaction parameters between (O2 ,Va), (O2 ,CsO2) and (CsO2,O) species are assessed to describe the liquidus in (Cs–Cs2O), (Cs2O–CsO2) and (CsO2–O) composition ranges, respectively. where yi are the constituent fractions. Their sum is thus unity. bij is the number of atoms j in the species i. The standard pressure p0 is set to 105 Pa. The partial pressure of species i, pi is related to the constituent fraction by pi = yi p where p is the total pressure. The thermodynamic parameters were taken from the SGTE substance database . C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 73 Table 5 Enthalpy of formation (ΔH0f), standard entropy (S0) and heat capacity (Cp0) data at 298.15 K for all the cesium oxide compounds. Comparison between calculated data (DFT and CALPHAD calculations from this work) and results coming from the literature (experiments, DFT and reviews). Oxide ΔH0f 298.15 K (kJ/mol) S0 298.15 K (J mol 1 K 1) Cp0 298.15 K (J mol 1 K 1) Method reference Cs7O 299.8 340.5 617.3 624.6 210.5 210.4 DFT – this work CALPHAD – this work Cs4O 298.2 339.2 304.3 364.2 136.4 128.7 DFT – this work CALPHAD – this work Cs7O2 from Cs11O3 576.0 682.3 545.0 621.4 231.2 231.1 DFT – this work CALPHAD – this work Cs3O 296.5 370.3 (0 K) 341.9 237.0 – 261.8 106.8 – 102.7 DFT – this work DFT – Jain CALPHAD – this work Cs2O 367.1 350.8 (0 K) 352.2 (0 K) – 346.0 346.0 346.0 346.0 348.4 346.0 157.3 – – 146.9 146.9 146.9 146.9 146.7 114.6 146.9 74.8 – – 76 – 76 – – – 75.7 DFT – this work DFT – Jain  DFT – Brillant  Exp. – Flotow  Rev. – Cordfunke  Rev. – SGTE  Rev. – Lamoreaux Exp. – Settle  Exp. – Knights  CALPHAD – this work Cs2O2 391.8 524.1 (0 K) 516.2 (0 K) 440.0 440.0 497.6 386.5 390.0 163.7 – – 173.6 180 144.3 213.3 215.4 111.0 – – – 95.0 – – 93.5 DFT – This work DFT – Jain  DFT – Brillant  Rev. – Cordfunke  Rev. – SGTE  Rev. – Lamoreaux  Exp. – Knights  CALPHAD – this work CsO2 252.8 388.6 (0 K) 351.2 (0 K) 233.1 286.2 286.2 234.9 241.4 147.5 – – 136.5 142.0 139.8 171.2 163.2 68.2 – – – 78.9 – – 68.45 DFT – this work DFT – Jain  DFT – Brillant  Rev. – Cordfunke  Rev. – SGTE  Rev. – Lamoreaux  Exp. – Knights  CALPHAD – this work CsO3 284.0 200.7 (0 K) 272.6 144.7 – 168.6 84.3 – 84.2 DFT – this work DFT – Jain  CALPHAD – this work 4.2. Optimization method The optimized Gibbs energy parameters for all the phases are reported in Table 4. As reported in Section 3.2, in a ﬁrst step, the c and dn coefﬁcients entering the Gibbs energy functions 0GiCsn Om for the oxide compounds (Eq. (9)) were ﬁxed by ﬁtting the calculated values from ab initio calculations combined with the quasi-harmonic thermodynamic model (Section 3, Table 3) for Cs7O, Cs4O, Cs3O, Cs7O2, Cs2O2, CsO2, and CsO3 oxides. For Cs2O compound, experimental data were preferred for the ﬁt. In a second step, the enthalpy and entropy terms for solid Cs2O were assessed. The a and b coefﬁcients in the Gibbs energy functions 0GiCsn Om in Eq. (9) were initialized considering the experimental enthalpy of formation and standard entropy at 298.15 K from respectively Settle et al.  and Flotow and Osborne . For liquid Cs2O, the melting enthalpy estimated by Lamoreaux and Hildenbrand  was utilized. In a third step, interaction parameters in the liquid between (O2 and Va) species were assessed to ﬁt experimental oxygen potential data measured in the Cs–Cs2O region by Knights and Phillips . Then the a and b coefﬁcients in the Gibbs energy functions 0GiCsn Om in Eq. (9) for Cs7O, Cs4O, Cs7O2, and Cs3O were assessed to ﬁt the phase diagram data in the Cs–Cs2O region. In a fourth step, the region between Cs2O and O was investigated. The a and b coefﬁcients in the Gibbs energy functions 0 Csn Om in Eq. (9) for Cs2O2 and CsO2 were assessed using oxygen Gi pressure data measured by Berardinelli [15,16]. As starting value, the melting enthalpy estimated by Lamoreaux and Hildenbrand  was taken for the Gibbs energy of CsO2 liquid. Finally, in a last step, interaction parameters in the liquid between (O2 ,CsO2) and (CsO2,O) were assessed to ﬁt the scarce phase diagram data in the Cs2O–O region. These experimental data correspond only to the melting points for Cs2O2, CsO2, and the decomposition temperature for CsO3. Oxygen potential data measured by Berardinelli  above the melt were also incorporated. It was not possible to lead to a good agreement for the melting point of Cs2O2, but as mentioned previously, the melting point for this compound is quite uncertain. 4.3. Results and discussion The calculated phase diagrams without and with the gas phase are presented in Fig. 1(a) and (b), respectively. 74 C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 Fig. 1. Calculated phase diagram of the Cs-O system (a) without gas phase (b) with gas phase. A good agreement between the calculated phase diagram and the experimental data is found in the Cs–Cs2O region, for which experimental information is available. As mentioned in the literature review, the phase diagram from Cs2O composition to pure oxygen is quite uncertain due to experimental issues. There are no liquidus data except the roughly value coming from Berardinelli . Only melting point values for Cs2O, Cs2O2, CsO2 and decomposition temperature for CsO3 are available in the literature. In the assessment, it was not possible to reproduce the melting point of Cs2O2 (863 K). By increasing the weighting factor to ﬁt the melting point for Cs2O2, at 863 K, the compound became unstable at room temperature and pressure data and thermodynamic data at room temperature were not well reproduced. Because the original paper on the determination of this melting point for Cs2O2 compound could not be found, no information is Fig. 2. (a) Calculated oxygen potential (J mol 1) versus temperature for 3.33, 4.65, 7.9, 10.3, 12.4, 16.8 at% O; (b) calculated oxygen and cesium chemical potential (J mol 1) versus oxygen atomic fraction at 773 K; comparison with experimental data measured by Knights and Phillips . available on this measurement, which is reported in previous papers. Thus, this value is considered as quite uncertain. Moreover, the most stable compound in the Cs-O system is Cs2O, which thus should have the highest melting point, instead of Cs2O2. Thus, a largest weighting factor was attributed to thermodynamic data on solid Cs2O2, which was derived from both ab initio and quasiharmonic model and from vapor pressure measurements above the (Cs2O þCs2O2) and (Cs2O2 þCsO2) regions. Fig. 2(a) compares calculated oxygen potential data versus temperature in the liquid (Cs–Cs2O region) to the experimental measurements by Knights and Phillips . Both calculated oxygen and cesium chemical potential data versus oxygen composition at 773 K are compared to data from Knights and Phillips  C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 75 Fig. 3. Calculated heat capacity data versus temperature using the regression laws reported in Table 3 and also used in the CALPHAD models for (a) Cs7O, (b) Cs4O, (c) Cs7O2, (d) Cs3O, (e) Cs2O, (f) Cs2O2, (g) CsO2, (h) CsO3 and comparison with the data calculated using the DFT and quasi-harmonic model (black points) as well as with data coming from the literature. in Fig. 2(b). A good agreement is obtained for both oxygen and cesium chemical potential, which gives a good conﬁdence in the thermodynamic model for the Cs–Cs2O region. Table 3 lists the Gibbs energy coefﬁcients for the compounds and the heat capacity, which were derived from ab initio calculations and quasi-harmonic model; except for Cs2O, which was directly ﬁtted from experimental data. Heat capacity data for all compounds are presented in Fig. 3(a)–(h). The comparison with data from the literature is only possible for Cs2O, Cs2O2, and CsO2. Experimental data only exist for the Cs2O compound. For this compound, the agreement between the model (ab-initio þ quasiharmonic approximation) and the experimental data measured by Flotow and Osborne  below 350 K is good, which gives conﬁdence to the results obtained by our approach. The estimation by Lamoreaux and Hildenbrand  is only valid for temperatures above 300 K and leads to systematically higher values for heat capacities at high temperature for Cs2O, Cs2O2, and CsO2. As no experimental data are available in this temperature range, our calculated functions using our approach (ab initio þquasi-harmonic approximation) are preferred. Once the heat capacity functions were ﬁxed for all the compounds, the enthalpy and entropy terms for Cs2O were assessed to ﬁt experimental data from Settle et al.  for the enthalpy of formation and from Flotow and Osborne  for the standard entropy at 298.15 K. Then the enthalpy and entropy terms for Cs2O2 and CsO2 were assessed to ﬁt oxygen pressure data 76 C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 Fig. 5. Calculated pressure data versus composition in Cs2O2–CsO2 region at 733, 753 and 773 K compared to the experimental data from Berardinelli . Fig. 4. Calculated pressure data versus temperature above (a) (Cs2Oþ Cs2O2) and (b) (Cs2O2 þ CsO2) regions, compared to the experimental data from Berardinelli [15,16] and Morris . measured by Berardinelli [15,16] above the (Cs2O þCs2O2) and (Cs2O2 þ CsO2) regions. As shown in Fig. 4(a) and (b), the agreement is very good between the calculated and experimental pressure data. For the liquid in the Cs2O–O region, melting enthalpy data estimated by Lamoreaux and Hildenbrand  for Cs2O and CsO2 were used to determine the Gibbs energy functions for these compositions in the liquid. Then interaction parameters between (O2 ,CsO2) and (CsO2,O) were assessed to try to reproduce the very tentative phase diagram proposed by Knights and Phillips . Oxygen pressure data measured in the melt close to the CsO2 composition were found in . It is surprising to note that these measurements were not reported in the published work by Fig. 6. Calculated enthalpy of formation for cesium oxides (J mol 1 at 1) compared to available literature data. Berardinelli  or Knights and Phillips . An attempt was made to ﬁt these experimental pressure data measured in both (liquid þCs2O2) and liquid regions. As shown in Fig. 4(b), a very good agreement is found for the pressure data versus temperature in the (liquid þ Cs2O2) region. Pressure data obtained in both (liquid þCs2O2) and liquid regions versus oxygen composition at 733, 753, and 773 K melt are compared to experimental data measured by Berardinelli  in Fig. 5. The order of magnitude of calculated pressure is correct (around 10 % at 733 and 753 K). The deviation is higher at 773 K in the liquid where experimental issues are expected. As this region of the phase diagram is very uncertain and thermodynamic data are scarce, we chose to assess a minimum number of interaction parameters. New experiments C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 Fig. 7. Calculated enthalpy of formation of cesium oxides in J mol 1 of O2. Table 6 Mulliken charge for cesium and oxygen ions, population bond and length for oxygen–cesium bond, calculated with CASTEP code for the cesium oxides. Bond population may be used to assess the covalent or ionic nature of a bond. A high value of the bond population indicates a covalent bond, while a low value indicates an ionic interaction. Oxide Cs7O Cs4O Cs11O3(Cs7O2) Cs3O Cs2O Cs2O2 CsO2 CsO3 Mulliken charge oxygen cesium 1.54 1.54 1.55 1.53 1.33 0.81 0.44 0.46 0.10–0.43 0.10–0.68 0.18–0.66 0.51 0.66 0.81 0.88 0.90 Population bond O–Cs Length (Å) O–Cs 0.07 0.10 0.10 0.06 0.40 0.22 0.00 0.00 2.78091 2.96546 2.98298 2.90607 2.85277 2.96074 2.97532 3.23100 on both the phase diagram in the Cs2O–CsO3 composition range and on thermodynamic data for Cs2O2, CsO2 and CsO3 would be very useful to better describe thermodynamics of the Cs–O system in this composition and temperature range. Standard enthalpy of formation, entropy, and heat capacity data at 298.15 K for all oxide compounds are reported in Table 5 and compared to available information. The calculated enthalpies of formation for all oxides are presented in Fig. 6 along side a comparison to available literature data. For Cs7O, Cs4O, Cs7O2, and Cs3O compounds, there are no literature data. In the Gibbs energy function, the enthalpy and entropy terms (a and b) were assessed to reproduce the phase diagram data, namely the decomposition temperature. The enthalpy of formation data obtained by DFT was not used in the assessment. The ﬁnal calculated enthalpy of formation data using the CALPHAD model are signiﬁcantly lower (12–16%) compared to the calculated data using DFT. This disagreement has no simple explanation in terms of ab initio calculations. It could be attributed to the reference energy of the free atoms in relation to the pseudopotential used to calculate the crystal cohesive energy, to the enthalpy increment between 0 K and the room temperature that the 77 thermodynamic model may overestimate. For Cs2O, Cs2O2, CsO2 and CsO3 compounds, the agreement between CALPHAD and DFT data is excellent (0.5–6%). Both calculated data are consistent with experimental data from Settle  and Knights  for Cs2O and from Knights  for Cs2O2 and CsO2 and with the review by Cordfunke . On the contrary, the assessed data by Lamoreaux and Hildenbrand , Lindemer  and in the Substance SGTE database  are underestimated. For the standard entropy at 298.15 K for Cs2O, the CALPHAD assessment reproduces selected experimental data from the calorimetric measurements by Flotow and Osborne . The entropy derived from the pressure measurements by Berardinelli [15,16] is quite low in comparison to the value determined from calorimetry  whereas the calculated value by ab initio is 7% too high. More conﬁdence was given to calorimetric measurements in agreement with Cordfunke . For Cs2O2 and CsO2, only experimental data derived from vapor pressure data by Berardinelli [15,16] was available. The agreement is very good between assessed data of Cs2O2 and reasonable for CsO2 and Knights . Estimates by Cordfunke and Konings , Lamoreaux and Hidenbrand , Lindemer  are quite low compared to our assessed data as well as the entropy data derived from ab initio and quasi-harmonic approximation. For the other oxide compounds, there are no experimental data. The assessed data with CALPHAD are systematically higher than DFT data. The calculated heat capacity of Cs2O at 298.15 K using CALPHAD or the DFT model is in good agreement with experimental data measured by Flotow , which gives a good conﬁdence to the model coupling DFT and quasi-harmonic calculations. Fig. 7 shows a different way to represent the calculated enthalpies of formation versus the oxygen mole fraction where these data are expressed in Joules for 1 mol of O2. For the metallic compounds Cs7O, Cs4O, Cs7O2 and Cs3O, these enthalpies do not substantially change with composition. This is due to the fact that oxygen is sufﬁciently diluted so that the electronic structure of the metal is just slightly disturbed: the oxygen Mulliken charge varies very little throughout the series as shown in Table 6. This is not the case for the insulators Cs2O, Cs2O2, CsO2  and CsO3. For these compounds, the oxygen–cesium bond population decreases and the cesium Mulliken charge increases from Cs2O to CsO3 (Table 6) indicating an increasing ionicity. On the contrary, the oxygen–cesium covalency is decreasing. Thus the oxide Cs2O is the most covalent compound, which is consistent as it is the most stable phase. It conﬁrms the fact that there is no reason for Cs2O2 to have a higher melting point than Cs2O as stated previously. New enthalpy of formation and heat capacity measurements would be very useful to better describe thermodynamics of the Cs–O system. 5. Conclusion A review of available data on thermodynamics and phase diagram data of the cesium–oxygen system was ﬁrst presented. Due to the lack of experimental thermodynamic data for the oxide compounds, ab initio calculations combined with a quasi-harmonic thermodynamic model were performed to estimate enthalpy of formation, standard entropy data and heat capacity data versus temperature for Cs7O, Cs4O, Cs7O2, Cs3O, Cs2O, Cs2O2, CsO2, and CsO3 oxides. This approach was successfully applied and validated on the Cs2O compound for which experimental data are available. Finally these calculated data coupled with available data coming from the literature were used to assess all the thermodynamic properties of the Cesium–Oxygen system using the CALPHAD method. A consist thermodynamic description of this system was 78 C. Guéneau, J.-L. Flèche / CALPHAD: Computer Coupling of Phase Diagrams and Thermochemistry 49 (2015) 67–78 obtained. The variation of thermodynamic data of the different oxides was related to their structural and bond properties investigated by ab-initio calculation. This work shows that the current approach combining CALPHAD and DFT/quasi-harmonic model is reliable and very useful, especially for such complex systems for which experiments are difﬁcult. Nevertheless experimental information is still missing on the phase diagram and particularly on the melting point of Cs2O2, which could not be reproduced by our model and suggest future measurements are warranted. This model will be used to model higher order chemical systems such as Cs–U–O, Cs–Mo–O, etc., as representative for phases that form in irradiated oxide fuels in nuclear reactors. Appendix A. Supplementary material Supplementary data associated with this article can be found in the online version at http://dx.doi.org/10.1016/j.calphad.2015.02.002. References  K. Konashi, T. Yato, H.H. Kaneko, J. Nucl. Mater. 116 (1983) 86.  C. Guéneau, B. Sundman, C. Chatillon, J. Nucl. Mater. 378 (2008) 257.  A. Berche, C. Rado, O. Rapaud, C. Guéneau, J. Rogez, J. Nucl. Mater. 389 (2009) 101.  A. Berche, N. Dupin, C. Guéneau, C. Rado, B. Sundman, J.-C. Dumas, J. Nucl. Mater. 411 (2011) 131.  C. Guéneau, N. Dupin, B. Sundman, C. Martial, J.-C. Dumas, S. Gossé, S. Chatain, F. De Bruycker, D. Manara, R.J.M. Konings, J. Nucl. Mater. 419 (2011) 145.  J.L. Flèche, Phys. Rev. B 65 (2002) 245116.  R.H. Lamoreaux, D.L. Hildenbrand, J. Phys. Chem. Ref. Data 13 (1984) 151.  E.H.P. Cordfunke, R.J.M. Konings, Thermochemical Data for Reactor Materials and Fission Products, Elsevier, North-Holland (1990) 92.  M.E. Rengade, Compt Rend., Acad. Sci 148 (1909) 1199.  G. Brauer, Z. Anorg. Allg. Chem. 255 (1947) 101.  C.F. Knights, B.A. Phillips, J. Nucl. Mater. 84 (1979) 196.  M. Blumenthal, M. Centerszwer, Bull Intern. Acad. Pol. Cl. Sci. Math. Nat. 1923 A (1933) 499.  I.I. Vol’nov, V.N. Belevskii, V.I. Klimanov, Izv. Akad. Nauk SSSR Ser. Khim. 7 (1967) 1411.  P. Touzain, J. Ther. Anal. 9 (1976) 441.  S.P. Berardinelli, Ph.D. thesis, University of Rhode Island, 1971.  S.P. Berardinelli, D.L. Kraus, Inorg. Chem. 13 (1974) 189.  H.E. Flotow, D.W. Osborne, J. Chem. Thermodyn. 6 (1974) 135.  G.V. Morris, Ph.D. thesis, University of Rhode Island, 1962.  M.N. Arnol’dov, M.N. Ivanovskii, G.N. Sereda, V.V. Stinikov, Russ. Metall. 4 (1975) 73.  J.L. Settle, G.K. Johnson, W.N. Hubbard, J. Chem. Thermodyn. 6 (1974) 263.  H. Okamoto, J. Phase Equilib. Diffus. 31 (2010) 86.  K.D. Hill, M. Gotoh, Metrologia 33 (1996) 307.  T.B. Lindemer, T.M. Besmann, J. Nucl. Mater. 100 (1981) 178.  J. Tai, Q. Ge, R.J. Davis, M. Neurock, J. Phys. Chem. B 108 (2004) 16798.  S. Gemming, G. Seifert, C. Mühle, M. Jansen, A. Albu-Yaron, T. Arad, R. Tenne, J. Solid State Chem. 178 (2005) 1190.  G. Brillant, F. Gupta, A. Pasturel, J. Phys.: Condens. Matter 21 (2009) 285602.  A. Jain, S.-A. Seyed-Reihani, C.C. Fischer, D.J. Couling, G. Ceder, W.H. Green, Chem. Eng. Sci. 65 (2010) 3025.  S. Riyadi, B. Zhang, R. de Groot, A. Caretta, P.H.M. van Loosdrecht, T.T.M. Pastra, G.R. Blake, Phys. Rev. Lett. 108 (2012) 217206.  S.J. Clark, M.D. Segall, C.J. Pickard, P.J. Hasnip, M.J. Probert, K. Refson, M. C. Payne, Z. Krist. 220 (2005) 567.  D. Vanderbilt, Phys. Rev. B 41 (1990) 7892.  J.P. Perdew, J.A. Chevary, S.H. Vosko, K.A. Jackson, M.R. Pederson, D.J. Singh, C. Fiolhais, Phys. Rev. B 46 (1992) 6671.  H.J. Monkhorst, J.D. Pack, Phys. Rev. B 16 (1977) 1748.  P. Villars, K. Cenzual, Pearson’s Crystal Data: Crystal Structure Database for Inorganic Compounds (on DVD), Release 2013/14, ASM Internationals, Materials Park, Ohio, USA, 2014.  F. Ortmann, F. Bechstedt, W.G. Schmidt, Phys. Rev. B 73 (2006) 205101.  A.T. Dinsdale, SGTE data for pure elements, CALPHAD 15 (4) (1991) 317.  M. Hillert, B. Jansson, B. Sundman, J. Agren, Metall. Trans. A 16 (1985) 661.  SGTE Substances Database, www.thermocalc.com/TCDATA.htm.  N. Beketov, Bull. Acad. Sci. Russ. 35 (1984) 541.
© Copyright 2022 Paperzz